- Nano Express
- Open Access
Graphitic carbon grown on fluorides by molecular beam epitaxy
Nanoscale Research Letters volume 8, Article number: 11 (2013)
We study the growth mechanism of carbon molecules supplied by molecular beam epitaxy on fluoride substrates (MgF2, CaF2, and BaF2). All the carbon layers form graphitic carbon with different crystallinities depending on the cation. Especially, the growth on MgF2 results in the formation of nanocrystalline graphite (NCG). Such dependence on the cation is a new observation and calls for further systematic studies with other series of substrates. At the same growth temperature, the NCG on MgF2 has larger clusters than those on oxides. This is contrary to the general expectation because the bond strength of the carbon-fluorine bond is larger than that of the carbon-oxygen bond. Our results show that the growth of graphitic carbon does not simply depend on the chemical bonding between the carbon and the anion in the substrate.
From the success of graphene growth on Ni or Cu by chemical vapor deposition (CVD) [1, 2], some variations were introduced to CVD to avoid the use of metallic catalysts [3–8]. However, the growth of carbon by chemical methods involves a complex mechanism due to the presence of carrier gases. For example, hydrogen acts as an etching reagent as well as a co-catalyst . In contrast, physical deposition methods such as molecular beam epitaxy (MBE) are useful to understand the growth mechanism of carbon because of the relatively simple kinetics [10–13]. Experimentally, it has been shown that nanocrystalline graphite (NCG) could be formed on crystalline and amorphous oxides by direct sublimation of carbon [14–16]. Although first-principles calculations partly explained that the strong bonding between carbon and oxygen limited the cluster size [14, 16], the growth mechanism is yet to be understood.
So far, carbon MBE has been tried on substrates containing elements from group IV [10–13], group V , and group VI [12, 14–16]. Here, we present the results of carbon MBE on fluorides (where the anion belongs to group VII) and compare them with similar studies on oxides to understand the effect of the anion on the quality of NCG. Since the bonding between carbon and fluorine is much stronger than the bonding between carbon and oxygen, we expected the carbon film to be more amorphous. On the contrary, NCG of good crystallinity was formed on MgF2, and the cluster size deduced from Raman spectra was even larger than those of NCGs on MgO and sapphire [18, 19]. These results show that the quality of NCG does not simply depend on the bond strength of carbon and substrate anion, and imply that the carbon growth mechanism could be more complex than previously thought.
Materials and film fabrication
Carbon MBE was done using a home-made ultra-high-vacuum MBE system and a carbon sublimation cell with a pyrolytic graphite filament. The pressure of the chamber was kept below 1.0×10−7 Torr during the growth by flowing liquid nitrogen in the shroud. Details about the growth procedure can be found elsewhere . Fluoride substrates (MgF2(100), CaF2(100), and BaF2(111)) were purchased from a commercial vendor (CrysTec GmbH, Berlin, Germany). The growth temperature was fixed at 900°C because of the lower melting points of fluoride substrates compared to oxides.
Raman scattering measurements and spatial mapping were performed using a micro-Raman spectroscope (inVia system, Renishaw, Wotton-under-Edge, UK) operated by a 514.5-nm laser. A minimal laser power of 2 mW was used during the measurements to avoid any damage or heating of the carbon films. Atomic force microscopy (AFM) images were taken by a commercial system (NanoFocus Inc., Seoul, South Korea) in a non-contact mode. AFM in a contact mode was also used to determine the film thickness by measuring the step height after lithography. X-ray photoelectron spectroscopy (XPS) measurements to analyze carbon bonding characteristics were done using a Kratos X-ray photoelectron spectrometer (Kratos Analytical Ltd, Manchester, UK) with Mg Kα X-ray source. C1s spectra were acquired at 150-W X-ray power with a pass energy of 20 eV and a resolution step of 0.1 eV.
Results and discussion
Figure 1 shows the Raman spectra from 3- to approximately 5-nm-thick carbon films grown on various fluorides by MBE. The characteristic peaks of graphitic carbon are well identified in all films: the D peak at approximately 1,350 cm−1 and the G peak at approximately 1,590 cm−1. These and previous studies show that MBE is an effective method for graphitic carbon growth on a wide range of substrates [14–17]. The degree of graphitization is, however, quite different depending on the cation. In fact, graphitic carbon refers to a wide range of disordered graphite, from NCG to mainly sp2 amorphous carbon. As clarified by Ferrari , the relative strength of D and G peaks alone cannot determine the degree of disorder, and it is the 2D peak at approximately 2,700 cm−1 which distinguishes NCG from amorphous carbon. As shown in Figure 1, the Raman spectra of the carbon film on MgF2 show a clear 2D peak, indicating that successful NCG growth was accomplished on MgF2 by carbon MBE. In contrast, the carbon films grown on CaF2 and BaF2 can be ascribed to amorphous carbon. As far as we know, carbon MBE on a family of substrates having the same anion has not been reported. Clear understanding of this cation dependence is yet to come, but our results will stimulate systematic studies on other series of substrates and further theoretical investigations.
We will focus on the growth on MgF2 from now on and compare the results with NCGs on oxides. For a quantitative comparison, the Raman spectra of NCG on MgF2 were fit by several Lorentzian functions as in  (Table 1). Interestingly, the intensity ratios of the D peak and 2D peak to the G peak (ID/IG and I2D/IG) are larger than those from NCG on MgO. Furthermore, all the peaks are narrower, implying a better crystallinity on MgF2 (from the comparisons of the full width at half maximum (FWHM) in Table 1 and those in ). The average cluster size, La, can be calculated from the relation ID/IG = C La2, where C = 0.0055 and La in Å . From ID/IG = 2.7 (Table 1), we get La = 22 Å, a slight increase from those on oxides [15, 16]. Figure 2 shows a Raman map of the intensity ratio of ID/IG over 10 μm2. Most regions have ID/IG = 2.7 ± 0.1, thus showing a high degree of uniformity. The uniformity is also better than that of NCG on MgO .
All these results indicate that NCG on MgF2 is less disordered than those on oxides. This is quite surprising if we consider the bond strength of the C-F bond, which is larger than the C-O bond strength [18, 19]. The high electronegativity of fluorine even makes the C-F bond partially ionic. From first-principles calculations, we have known that the strong C-O bond limits the cluster size of NCG on sapphire and MgO [14, 16]. If that is the whole story, the stronger C-F bond should lead to smaller clusters on MgF2. Our results against this imply that an important factor is missing in the theoretical understanding of the NCG growth mechanism. Recently, models such as the catalytic role of step edges or the migration of cyclic carbons are good examples of pertinent suggestions [4, 21].
Figure 3 presents XPS results to clarify the carbon bonding characteristics. Similar to previous studies [14, 16], 284.7 ± 0.2 and 285.6 ± 0.2 eV components in C1s spectra are attributed to sp2 and sp3 bonds , namely, sp2 hybridization of carbon atoms and sp3 hybridization of C-C or C-H bonds, respectively . The fitting results show that the fraction of the sp2 bond is more than 80%, confirming the NCG formation on MgF2.
Finally, Figure 4 shows AFM images before and after the NCG growth on MgF2. Unlike crystalline and amorphous oxide substrates, the mean roughness parameter, Ra, of the MgF2 substrate is large. The Ra of NCG (2.45 nm over 1 × 1 μm scan) is even larger by an order of magnitude than those NCGs on oxide substrates [14–16]. It is not clear why the surface morphology is worse while the Raman spectra indicate a better crystallinity. We hope that the understanding of NCG growth on MgF2 can lead to better NCG or possibly graphene growth on other (flat) dielectrics.
In summary, we have grown graphitic carbon on fluoride substrates, expanding the application of carbon MBE into group VII anions. While amorphous carbons were formed on CaF2 and BaF2, nanocrystalline graphite of good crystallinity was formed on MgF2 despite the strong bonding between carbon and fluorine. In comparison to similar studies on MgO, the effect of the substrate anion on the quality of NCG contradicts the expectation based on the bond strength between carbon and the anion. Further systematic studies and theoretical investigations are encouraged to understand the carbon growth mechanism by MBE.
Atomic force microscopy
Chemical vapor deposition
The full width at half maximum
Molecular beam epitaxy
X-ray photoelectron spectroscopy.
Kim KS, Zhao Y, Jang H, Lee SY, Kim JM, Kim KS, Ahn J-H, Kim P, Choi J-Y, Hong BH: Large-scale pattern growth of graphene films for stretchable transparent electrodes. Nature 2009, 457: 706–710. 10.1038/nature07719
Li X, Cai W, An J, Kim S, Nah J, Yang D, Piner R, Velamakanni A, Jung I, Tutuc E, Banerjee SK, Colombo L, Ruoff RS: Large-area synthesis of high-quality and uniform graphene films on copper foils. Science 2009, 324: 1312–1314. 10.1126/science.1171245
Su CY, Lu AY, Wu CY, Li YT, Liu KK, Zhang W, Lin SY, Juang ZY, Zhong YL, Chen FR, Li LJ: Direct formation of wafer scale graphene thin layers on insulating substrates by chemical vapor deposition. Nano Lett 2011, 11: 3612–3616. 10.1021/nl201362n
Scott A, Dianat A, Borrnert F, Bachmatiuk A, Zhang SS, Warner JH, Borowiak-Palen E, Knupfer M, Buchner B, Cuniberti G, Rummeli MH: The catalytic potential of high-kappa dielectrics for graphene formation. Appl Phys Lett 2011, 98: 073110. 10.1063/1.3556639
Kidambi PR, Bayer BC, Weatherup RS, Ochs R, Ducati C, Szabó DV, Hofmann S: Hafnia nanoparticles – a model system for graphene growth on a dielectric. Phys Status Solidi Rapid Res Lett 2011, 5: 341–343. 10.1002/pssr.201100155
Song HJ, Son M, Park C, Lim H, Levendorf MP, Tsen AW, Park J, Choi HC: Large scale metal-free synthesis of graphene on sapphire and transfer-free device fabrication. Nanoscale 2012, 4: 3050–3054. 10.1039/c2nr30330b
Bi H, Sun SR, Huang FQ, Xie XM, Jiang MH: Direct growth of few-layer graphene films on SiO2 substrates and their photovoltaic applications. J Mater Chem 2012, 22: 411–416. 10.1039/c1jm14778a
Medina H, Lin YC, Jin CH, Lu CC, Yeh CH, Huang KP, Suenaga K, Robertson J, Chiu PW: Metal-free growth of nanographene on silicon oxides for transparent conducting applications. Adv Funct Mater 2012, 22: 2123–2128. 10.1002/adfm.201102423
Vlassiouk I, Regmi M, Fulvio PF, Dai S, Datskos P, Eres G, Smirnov S: Role of hydrogen in chemical vapor deposition growth of large single-crystal graphene. ACS Nano 2011, 5: 6069–6076. 10.1021/nn201978y
Hackley J, Ali D, DiPasquale J, Demaree JD, Richardson CJK: Graphitic carbon growth on Si(111) using solid source molecular beam epitaxy. Appl Phys Lett 2009, 95: 133114. 10.1063/1.3242029
Al-Temimy A, Riedl C, Starke U: Low temperature growth of epitaxial graphene on SiC induced by carbon evaporation. Appl Phys Lett 2009, 95: 231907–231907–3.
Maeda F, Hibino H: Thin graphitic structure formation on various substrates by gas-source molecular beam epitaxy using cracked ethanol. Jpn J Appl Phys 2010, 49: 04DH13–04DH13–6.
Moreau E, Godey S, Ferrer FJ, Vignaud D, Wallart X, Avila J, Asensio MC, Bournel F, Gallet JJ: Graphene growth by molecular beam epitaxy on the carbon-face of SiC. Appl Phys Lett 2010, 97: 241907. 10.1063/1.3526720
Jerng SK, Yu DS, Kim YS, Ryou J, Hong S, Kim C, Yoon S, Efetov DK, Kim P, Chun SH: Nanocrystalline graphite growth on sapphire by carbon molecular beam epitaxy. J Phys Chem C 2011, 115: 4491–4494.
Jerng SK, Yu DS, Lee JH, Kim C, Yoon S, Chun SH: Graphitic carbon growth on crystalline and amorphous oxide substrates using molecular beam epitaxy. Nanoscale Res Lett 2011, 6: 565. 10.1186/1556-276X-6-565
Jerng SK, Lee JH, Yu DS, Kim YS, Ryou J, Hong S, Kim C, Yoon S, Chun SH: Graphitic carbon growth on MgO(100) by molecular beam epitaxy. J Phys Chem C 2012, 116: 7380–7385. 10.1021/jp210910u
Jerng SK, Yu DS, Lee JH, Kim YS, Kim C, Yoon S, Chun SH: Carbon molecular beam epitaxy on various semiconductor substrates. Mater Res Bull 2012, 47: 2772–2775. 10.1016/j.materresbull.2012.04.123
O'Hagan D: Understanding organofluorine chemistry. An introduction to the C-F bond. Chem Soc Rev 2008, 37: 308–319. 10.1039/b711844a
Lemal DM: Perspective on fluorocarbon chemistry. J Org Chem 2004, 69: 1–11. 10.1021/jo0302556
Ferrari AC: Raman spectroscopy of graphene and graphite: disorder, electron–phonon coupling, doping and nonadiabatic effects. Solid State Comm 2007, 143: 47–57. 10.1016/j.ssc.2007.03.052
Lippert G, Dabrowski J, Yamamoto Y, Herziger F, Maultzsch J, Lemme MC, Mehr W, Lupina G: Molecular beam growth of micrometer-size graphene on mica. Carbon 2013, 52: 40–48.
Ermolieff A, Chabli A, Pierre F, Rolland G, Rouchon D, Vannuffel C, Vergnaud C, Baylet J, Semeria MN: XPS, Raman spectroscopy, X-ray diffraction, specular X-ray reflectivity, transmission electron microscopy and elastic recoil detection analysis of emissive carbon film characterization. Surf Interface Anal 2001, 31: 185–190. 10.1002/sia.955
Luo Z, Yu T, Kim K-j, Ni Z, You Y, Lim S, Shen Z, Wang S, Lin J: Thickness-dependent reversible hydrogenation of graphene layers. ACS Nano 2009, 3: 1781–1788. 10.1021/nn900371t
This research was supported by the Priority Research Centers Program (2012–0005859), the Basic Science Research Program (2012–0007298, 2012–040278), the Center for Topological Matter in POSTECH (2012–0009194), and the Nanomaterial Technology Development Program (2012M3A7B4049888) through the National Research Foundation of Korea (NRF) funded by the Ministry of Education, Science and Technology (MEST).
The authors declare that they have no competing interests.
SKJ carried out the carbon molecular beam epitaxy experiments and X-ray photoelectron spectroscopy. JHL carried out the atomic force microscopy measurements. YSK characterized the thin films by Raman spectroscopy. SHC designed the experiments and wrote the manuscript. All authors read and approved the final manuscript.
About this article
Cite this article
Jerng, SK., Lee, J.H., Kim, Y.S. et al. Graphitic carbon grown on fluorides by molecular beam epitaxy. Nanoscale Res Lett 8, 11 (2013). https://doi.org/10.1186/1556-276X-8-11
- Graphitic carbon
- Molecular beam epitaxy